| ||Format||Pages||Price|| |
|4||$56.00||  ADD TO CART|
Formerly under the jurisdiction of Committee B07 on Light Metals and Alloys, this test method was withdrawn in October 2013. This standard is being withdrawn without replacement because (1)the standard covers one particular instrument that is no longer available from the manufacturer, and (2) comparative test data show that the reproducibility is inadequate.
1.1 This test method covers indentation hardness testing of aluminum alloys using a Newage, portable, non-caliper-type, hardness instrument which provides readout values numerically equivalent to Rockwell B-scale as determined by Test Methods E 18.Note 1
This is a comparative Rockwell B test and does not provide an actual Rockwell B test value. HRBN, the values obtained from the Newage instrument, are numerically equivalent to Rockwell B values, but do not represent an actual Rockwell B test in accordance with Test Methods E 18.
1.2 This test method measures indentation hardness of heat-treatable aluminum alloys having a hardness from 30 to 100 HRBN, a thickness greater than 1.50 mm (0.060 in.), and pieces too large to be tested by a caliper type instrument.Note 2
This test method covers two instruments (one analog and one digital) which operate differently. Refer to the manufacturer's instruction for proper operation.
1.3 The flat surface size of the area being tested must be compatible with the instrument support area and the material must not deflect during the test.
1.4 The values stated in SI units are the standard. The values given in parentheses are for information only.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
B648 Test Method for Indentation Hardness of Aluminum Alloys by Means of a Barcol Impressor
E18 Test Methods for Rockwell Hardness of Metallic Materials
E177 Practice for Use of the Terms Precision and Bias in ASTM Test Methods
E691 Practice for Conducting an Interlaboratory Study to Determine the Precision of a Test Method
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM B724-00(2006), Standard Test Method for Indentation Hardness of Aluminum Alloys by Means of a Newage, Portable, Non-Caliper-Type Instrument (Withdrawn 2013), ASTM International, West Conshohocken, PA, 2006, www.astm.orgBack to Top